Biomedical applications of inorganic nanoparticles:
Magnetic Resonance Imaging and Hyperthermia
Jesus Penaranda Avila
Submitted for the degree of Doctor of Philosophy
at the University of Milano-Bicocca
School of Doctorate in Nanotechnologies and Nanostructures
University of Milano-Bicocca
I List of abbreviations
AC Alternating current AMF Alternating magnetic field B Magnetic induction BBB Blood-brain barrier bp Boiling point
BSA Bovine serum albumin CH3COOH Acetic acid
CLIO Crosslinked iron oxide CoFe2O4 Cobalt ferrite
CTAB Cetyl trimethylammonium bromide DLS Dynamic light scattering
DMF Dimethyl formamide DMSO Dimethyl sulfoxide
DMEM Dulbecco’s Modified Eagle’s medium (cell cultures) DNA Deoxyribonucleic acid
EDC 1-Ethyl-3-(3-dimethylaminopropyl)carbodiimide EDTA Ethylenediaminetetraacetic acid
EGFR Epidermal growth factor receptor EPR Enhanced permeation and retention effect EtOH Ethanol
Et2O Diethyl ether
FACS Fluorescence Activated Cell Sorting (in this) FeCo Iron cobalt allow
FePt Iron platinum allow
FDA Food and drug Administration FBS Fetal bovine serum
Fe3O4 Magnetite γ-Fe2O3 Maghemite
FITC Fluorescein isothiocyanate
FT-IR Fourier Transform Infra-Red spectra
Gd2O3 Gadolinium oxide
Gd-DOTA Gd-tetraazacyclododecanetetraacetic acid Gd-DTPA Gd-diethylenetriamine pentaacetate GdF3 Gadolinium fluoride
GdPO4 Gadolinium phosphate H Magnetic field Hc Coercive field HCl Hydrochloridic acid
HER2 Human Epidermal growth factor receptor 2 HSA Human serum albumin
IBD Inflammatory bowel disease IPTES 3-isocyanatepropyl triethoxy silane ICAM1 Intercellular adhesion molecule 1 IONPS Iron oxide nanoparticles
IACUC Institutional Animal Care and Use Committee K Kelvin (unit for temperature)
Ku Anisotropy constant
MAdCAM1 Mucosal vascular addressin cell adhesion molecule 1 mAb Monoclonal antibody
II mM Millimolar concentration
μM Micromolar concentration
MCF7 Michigan Cancer Foundation-7; HER2 positive breast cancer cell line MEMRI Manganese-enhanced MRI
MPIO Paramagnetic iron oxide nanoparticles of micrometric size MNPs Magnetic nanoparticles
Mn-DPDP Mangafodipirtrisodium MnFe2O4 Manganese ferrite MnO Manganese oxide
MRI Magnetic resonance imaging
MTT 3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazolium bromide MPH Magnetic particle hyperthermia
Ms Saturation magnetization MR Remanent magnetization Mz Net Magnetization NaOH Sodium hydroxide
NSF Nephrogenic systemic fibrosis NHS N-hydroxysuccinimide NMR Nuclear magnetic resonance NaH Sodium hydride
NPs Nanoparticles NTA Nitrilotriacetic acid
NUS National University of Singapore PBS Phosphate buffer solution PEG Poly ethylene glycol PLGA Polylactide-co-glycolide acid
PMA Poly(isobutylene-alt-maleic anhydride) PVP Polyvinyl pyrrolidone
RNA Ribonucleic acid
RES Reticulo endothelial system rSP Superparamagnetic radius RF Radio frequency RT Room temperature σ Polidispersity
SAR Specific absorption rate SBB Sodium borate buffer scFV Portion of the whole antibody SBIC Singapore Bioimaging Consortium SEM Scanning electron microscopy SLP Specific loss power
SPIO Super paramagnetic iron oxide nanoparticles SPDP 3-(2-pyridyldithio)propionate
TE Echo time
TEM Transmission electron microscopy TEOS Tetraethyl orthosilicate
THF Tetrahydrofurane TR Repetition time
TZ Trastuzumab moloclonal antibody T1 Longitudinal relaxation
T2 Trasversal relaxation
USPIO Ultra small superparamagnetic iron oxide nanoparticles U87MG Human primary glioblastoma cell line
VEGF Vascular endothelial growth factor
I would like to thanks all the people who made possible this work, for their support and encouragement during these years. First of all, my gratitude goes to my supervisor, Dr. Davide Prosperi, for opening the doors of the NanoBioLab and giving me the opportunity of working with him and with all the wonderful persons who take part of his team; for being my mentor and for supporting me all the time.
Special thanks to Dr. Kai-Hsiang Chuang and Dr. Prashant Chandrasekharan, from SBIC, for giving me the tools to widen my skills in MRI during my stay in Singapore.
Thanks to the persons who collaborated and contributed with this work; all the team from Luigi Sacco Hospital and Nerviano Medical Sciences in Milan, and all the people from Prof. Ding’s lab at the National University of Singapore.
Inorganic nanoparticles have been extensively used in biomedical applications as a result of their electronic, optical, and magnetic properties that are derived from their nanometer size and composition. Their magnetic characteristics are crucial for the successful performance in applications such as magnetic resonance imaging (MRI), drug delivery, cellular signaling, and hyperthermia. MRI is one of the most powerful imaging techniques for living organisms as it provides images with excellent anatomical details based on soft-tissue contrast and functional information in a non-invasive and real-time monitoring manner. Among the different kinds of contrast agents currently available for clinical diagnosis, Gd-based contrast agents, specifically Gd (III) chelates, are used as positive magnetic resonance imaging (MRI) contrast agent. However, they generally induce the risk of nephrogenic systemic fibrosis (NSF) due to the dissociated Gd3+ ions from Gd (III) chelates. To avoid this problem, novel positive MRI contrast agents based on MnO have been developed, allowing low toxicity, high sensitivity, and active targeting when conjugated with biomolecules (antibodies).
During this work, the synthesis and characterization of MnO nanoparticles as positive contrast agents (T1) for MRI were carried out. Differences in size and morphology (round, star-like, cubic)
were found by varying the reaction parameters such as solvent, temperature and reaction time. In order to determine their contrast enhancement, T1-weighted images were acquired in vitro at
different concentrations. Furthermore, to study their biocompatibility, up-take and proliferation assays were done in culture of endothelial cells SVEC4-1. To assess their biodistribution and wash out time, studies in vivo were carried out using a colitis induced murine model with 3% Dextran Sodium Sulfate (DSS) in drinking water. Data acquired showed a selective accumulation to inflammatory site in a short time suggesting a potential applicability for the diagnosis of the Inflammatory Bowel Disease (IBD).
For that reason, in an attempt to develop nanoparticles with high thermal energy transfer capability, during my internship at the Singapore Bioimaging Consortium (SBIC) and in collaboration with NUS, it was carried out a project to assess the thermal efficiency of Gd doped iron oxide nanoparticles. By using MRI, T1 maps were obtained using a turbo-spin echo
VI List of publications
1. P. Verderio, S. Avvakumova, G. Alessio, M. Bellini, M. Colombo, E. Galbiati, S. Mazzucchelli, J. Peñaranda Avila, B. Santini, D. Prosperi. Delivering colloidal
nanoparticles to mammalian cells: a nano-bio interface perspective. Adv. Healthcare Mat.
2014, 3(7): 957-976.
2. E. Cova, M. Colombo, S. Inghilleri, M. Morosini, S. Miserere, J. Peñaranda-Avila, B. Santini, D. Piloni, S. Magni, F. Gramatica, D. Prosperi, F. Meloni. Antibody-engineered
nanoparticles selectively inhibit mesenchymal cells isolated from patients with chronic lung allograft rejection. Nanomedicine 2015, 10(1): 9-23.
3. S. Sommaruga, E. Galbiati, J. Peñaranda-Avila, C. Brambilla, P. Tortora, M. Colomobo, D. Prosperi. Immobilization of carboxypeptidase from Sulfolobus solfataricus
on magnetic nanoparticles improves enzyme stability and functionality in organic media.
Chapter I. Inorganic nanoparticles 4
1.1. Introduction 4
1.2. Magnetic nanoparticles 5
1.2.1. M–H curves 6
1.3. Iron oxide nanoparticles 8
1.3.1. Synthesis of iron oxide nanoparticles 9
22.214.171.124. Coprecipitation 10
126.96.36.199. Aerosol-vapor technology 10
188.8.131.52. Solvothermal decomposition from organo-metallic precursors 11 1.3.2. Applications of Iron Oxide Nanoparticles in Biomedical Research 12
184.108.40.206. Drug delivery 12
220.127.116.11. Nanosensors 13
18.104.22.168. Magnetic Resonance Imaging (MRI): T2 and T1 contrast agent 13
22.214.171.124. Hyperthermia 14
1.4. Manganese oxide nanoparticles 15
1.4.1. Synthesis of manganese oxide nanoparticles 15
1.4.2. Applications of Manganese oxide Nanoparticles in Biomedical Research 16
Chapter II. Magnetic resonance imaging 24
2.1. Relaxation times T1 and T2 26
2.1.1. T1-weighted images and Repetition Time (TR) 29
2.1.2. T2-weighted images and echo time (TE) 29
2.1.3. Magnetic Susceptibility 30
2.2. MRI contrast agents based on magnetic nanoparticles 31
2.2.1 Surface biocompatibility 32
2.3. T2 contrast agents 36
2.3.1. Nanostructured T2 contrast agents with improved magnetic properties 39
2.3.2. Multifunctional T2 contrast agents 41
2.4. T1 contrast agents 43
2.4.1 Gadolinium based contrast agents 45
2.4.2 New contrast agents based on Manganese 46
4 CHAPTER I
INORGANIC NANOPARTICLES 1.1. Introduction
The nanoscale, defined by the US National Nanotechnology Initiative, is a range from 1 to 1000 nm, including particles which are naturally occurring, such as particles in smoke, volcanic ash, sea spray, and from anthropogenic sources. In terms of biology, the nanoscale is the size range of important cellular components, such as double-stranded DNA (about 2.5 nm in diameter), proteins (hemoglobin is about 5 nm in diameter), cell walls, cell membranes, and compartments. The SI prefix “nano” means a billionth (10−9) part of a meter, or about one hundred thousandth the thickness of a sheet of paper.
Metal nanoparticles have a long history in terms of preparation, characterization, and application. Understanding and exploring their properties and potential applications are major driving forces behind the synthesis of a large variety of functional nanomaterials. Many of these properties arise from their large surface-area-to-volume ratio and the spatial confinement of electrons, phonons, and electric fields in and around the particles. These may cause deviations from the usual bulk atomic arrangements, such as higher reactivity; different elastic, tensile, and magnetic properties; increased conductivity; or increased tendency to reflect and refract light.
Nanoparticle research has been exploited to the use of inorganic nanoparticles in different technological fields; particularly, a significant factor is the development of a great number of applications in biomedical science, ranging from imaging to biochemical sensing, targeting and drug delivery.[3-9].
The main advantage of inorganic nanoparticles is attributed to their intrinsic physical properties including size dependent optical, magnetic, electronic, and catalytic properties as well as some biological activities (e.g. anti-bacteria or specific interactions). In addition, the possibility of
Moreover, many functional groups providing a wide range of potential interactions between organic moieties and biomolecules with nanoparticle surface can be easily used to compose a bio-nano structure with a specific biological function. Thus, the modification of peptides, proteins and other complex molecules with specific anchoring groups facilitates the binding to nanoparticles via a site-specific linkage, introducing chemical functionalities that can provide recognition of antibodies or cell receptors.. Understanding the profile of the biomolecule-nanoparticle interactions at their interface and with biological systems such as cells and tissues is crucial as it may affect the structures at the molecular level thus affecting their biological function or application. For that reason, design and optimization of effective functionalization strategies are critical to ensure the success of these nano-bio systems.
The present chapter focuses on describing some inorganic magnetic nanoparticles, specifically those based on iron (Fe) and manganese (Mn), which are promising for biomedical applications due to their fascinating properties. Different synthetic approaches of these nanoparticles will also be mentioned as well as their surface modifications with organic and active biomolecules.
1.2. Magnetic nanoparticles
6 1.2.1. M–H curves
Under the presence of a magnetic field of strength H, the individual atomic moments of a magnetic material contribute to its overall response so that the magnetic induction is defined by:
𝑩 = 𝝁𝟎(𝑯 + 𝑴), eq. (1)
where μ0 is the permeability of free space, and the magnetization M = m/V is the magnetic
moment per unit volume, where m is the magnetic moment on a volume V of the material. Since all materials are magnetic to some extent, with their response depending on their atomic structure and temperature, they may be conveniently classified in terms of their volumetric magnetic susceptibility, χ, where
𝑴 = 𝝌𝑯, eq. (2)
describes the magnetization induced in a material by H. In SI units χ is dimensionless and both M and H are expressed in Am−1. The susceptibility in ordered materials depends not just on temperature, but also on H, which gives rise to the characteristic sigmoidal shape of the M–H curve, with M approaching a saturation value at large values of H (Fig 1.1. a).
Magnetic materials are characterized by the presence of magnetic dipoles generated by the spinning of some of their electrons. Each of these polarized electrons can be aligned in a parallel or anti-parallel fashion with respect to the neighboring ones in the crystal lattice and this type of interaction is what gives rise to the macroscopic magnetic effect that we can measure. Depending on the magnetic response observed, it is possible to classify magnetic materials as paramagnets,
ferromagnets, ferrimagnets or anti-ferromagnet.
Paramagnetic materials are characterized by uncouple (randomly oriented) magnetic dipoles,
which can be aligned only in the presence of an external magnetic field and along its direction. This type of material has no coercivity nor remanence, which means that when the external magnetic field is switched off, the internal magnetic dipoles randomize again, no extra energy is required to demagnetize the material and hence the initial zero net magnetic moment is spontaneously recovered.
(a) Coercive Field (HC): is the external field of opposite sign required to reduce the
magnetization back to zero. It represents also the minimum energy required for the reversal of the magnetization of the material. HC is strictly related to the magnetic anisotropy constant (Ku)
that determines the energy to be overcome in order to invert the direction of the magnetic dipoles of the material and can have different contributions such as the symmetry of the crystal lattice, the surface contribution with respect to the core of the nanoparticle, and finally the shape of the nanoparticle.
(b) Saturation Magnetization (MS): is the maximum value of magnetization that the material can
reach under the effect of sufficiently high magnetic fields.
(c) Remanent Magnetization (MR): indicates the residual magnetization at zero applied field.
Figure 1.1: a) Theoretical magnetization (M) versus magnetic field (H) for different materials: Depending on the
particle size, materials exhibit either a multi-domain (green), single-domain (blue) or superparamagnetic (red) behavior. b) Variation of the coercivity (HC) of magnetic nanoparticles with size.
In materials where neighboring magnetic dipoles align anti-parallel in the lattice, thus repulsing each other, the magnetic exchange can led to two different phenomena called
anti-ferromagnetism and ferrimagnetism. The former case occurs when the magnetic dipoles or
interacting spins have the same value and hence the material shows a net zero magnetization. In the latter, the two coupled spins show different values so that the net magnetic dipole different than zero will still magnetize the material even in the absence of an external magnetic field.
To overcome the barrier to domain wall motion in these materials, energy is needed. This energy is delivered by the applied field, and can be characterized by the area enclosed by the hysteresis loop. This leads to the concept that applying a time-varying magnetic field to a ferromagnetic or ferrimagnetic material, it is possible to establish a constant flow of energy into that material, which will be transferred into thermal energy. The shape of these loops are determined in part
by particle size: in large particles (of the order micron size or more) there is a multi-domain ground state which leads to a narrow hysteresis loop since it takes relatively little field energy to make the domain walls move; while in smaller particles there is a single domain ground state which leads to a broad hysteresis loop. A further reduction of the size below a certain value of the radius (called superparamagnetic radius, rSP), induces a magnetic transition in particles where both ferro and ferrimagnetic nanoparticles become superparamagnetic. This behavior is strictly associated to nanoformed magnetic materials and arises when the thermal energy is sufficiently high to overcome the magnetic stabilization energy of the particle (Fig 1.1.b).
The size reduction of magnetic materials shows enhancing advantages that make them more suitable for therapeutic and diagnostic techniques compared to their bulk counterparts; for example magnetic parameters such as the HC of particles can be tuned by decreasing their size
and, consequently, the biomedical performance of the sample can be optimized to the practical requirements. This last property translates into a considerable advantage, especially for in vivo experiments: the absence of HC (the zero net magnetic moment) of the nanoparticles after
concluding the diagnostic measurement will prevent the potential aggregation of MNPs that could easily cause the formation of embolisms in the blood vessels.
1.3. Iron oxide nanoparticles
Iron is one of the most abundant metallic elements in living organisms, and is essential for various biological processes, such as oxygen transport by hemoglobin and cellular respiration by redox enzymes.
The application of small iron oxide particles in in vitro diagnostics has been practised for nearly 40 years. In the last decade, increased investigations with several types of iron oxides have been carried out in the field of nanosized magnetic particles (mostly maghemite, γ-Fe2O3, or magnetite,
Fe3O4, single domains of about 5–20 nm in diameter), among which magnetite is a very
promising candidate since its biocompatibility has been already proven . IONPs doped with magnetically susceptible elements (e.g. MnFe2O4 and CoFe2O4) and metal alloys nanoparticles
(e.g. FeCo and FePt) are also available, but they are much less employed in biomedical applications because of their potential toxicity and rapid oxidation, even though the magnetism of these ferrites and metal alloys is stronger than that of the corresponding pure iron oxide.
The metabolism and pharmacokinetics of intravenously injected IONPs have been well studied and, in addition to their superior biocompatibility, they offer many important advantages for biomedical applications, such as MRI contrast enhancement, tissue repair, immunoassays, detoxification of biological fluids, hyperthermia, drug delivery and cell separation. All of these applications require that the nanoparticles have high magnetization values, a size smaller than 100 nm, and a narrow particle size distribution. Moreover, the surface coating of these nanoparticles has to be nontoxic and biocompatible and must also allow for a targetable delivery with particle localization in a specific area. Such magnetic nanoparticles can bind to drugs, proteins, enzymes, antibodies, or nucleotides and can be directed to an organ, tissue, or tumor using an external magnetic field. Currently, there are some iron oxide nanoparticle-based MR contrast agents that have already been used in clinical trials, or are undergoing clinical trials . Most of them are covered by a specific organic and/or inorganic layer. Their appropriate coating depends on the type of nanoparticle core and the proposed applications since differently coated iron oxide nanoparticles will have different effects on cells and different fates in the body. Hence, the suitable chemical design of both the core and shell of the nanoparticle is extremely important for future projected clinical practice.
1.3.1. Synthesis of iron oxide nanoparticles
A great number of physical and chemical methods have been applied to synthesize MNPs.
To overcome these drawbacks, various chemical methods based on solution-phase colloidal chemistry have been investigated for the synthesis of high quality nanoparticles. These chemical methods include metal salt reduction, sol-gel process, reverse micelle technique, and thermal decomposition of iron organic precursors. Nevertheless, to prepare iron oxide nanoparticles suitable for the intended medical applications, the use of “green chemistry” is highly recommended, which avoids the use of toxic chemicals. It is also desirable to have a synthetic process that is scalable to industrial applications, and should be reproducible from batch to batch. A briefly description of the most representative methods for the scalable synthesis of iron oxide nanoparticles for medical use is described below.
126.96.36.199 - Coprecipitation
Magnetite is prepared by reacting Fe(II) and Fe(III) salts in alkaline aqueous media in a molar ratio of 1:2. Nanoparticles made by this method could be used for biomedical applications because of their easy and large-scale production; and their direct dispersion in water without further treatment. However, the synthesized magnetite particles from this process are highly
polydisperse and unstable. To further improve their stability, iron oxide nanoparticles were coated in situ using various capping ligands such as hydroxamate, dimercaptosuccinic acid, phosphorylcholine, and citric acid.[25, 26] However, the crystallinity of the synthesized iron oxide nanoparticles is very poor, which reduces their magnetic susceptibility.
188.8.131.52- Aerosol-vapor technology
184.108.40.206- Solvothermal decomposition from organo-metallic precursors
Highly uniform-disperse IONPs can be synthesized on a large scale by solvothermal decomposition of organometallic iron precursor such as iron pentacarbonyl, iron cupferron, iron oleate, or iron acetylacetonate in a hot surfactant solution.[29-33] Nanoparticles synthesized by solvothermal decomposition have high crystallinity and uniform size distribution with polidispersity (σ) ≈ 10%. Hyeon et al. reported the fabrication of highly uniform iron oxide nanoparticles by the thermal decomposition of iron oleate complex, which was prepared by the reaction of iron pentacarbonly with oleic acid. Monodisperse iron oxide nanoparticles were
obtained by mixing iron pentacarbonly precursor with oleic acid solution at low temperature and heating up the reaction mixture to high temperature. The size of the nanoparticles was controlled by adjusting the molar ratio of iron pentacarbonyl to oleic acid. Few years later it was reported a synthetic method of obtaining mono-disperse IONPs using an inexpensive and nontoxic iron chloride (FeCl3) rather than toxic and expensive iron pentacarbonyl; (Figure. 1.2).
Figure 1.2: Scheme for the ultra-large-scale synthesis of monodisperse nanocrystals.
A dispersion containing the iron-oleate complex, generated from the reaction between FeCl3 and
This size could be finely controlled from 1.5 nm to 3.7 nm by changing the ratio of oleyl alcohol to oleic acid or by changing the aging temperature.[2, 38]
1.3.2. Applications of Iron Oxide Nanoparticles in Biomedical Research
Magnetic nanoparticles offer some attractive possibilities in biomedicine. Their controllable sizes ranging from a few nanometers up to tens of nanometers, places them at dimensions where they can ‘get close’ to a biological entity of interest. Indeed, they can be coated with biological molecules to make them interact with or bind to a biological entity, thereby providing a controllable means of ‘tagging’ or addressing it. In this section four particular applications of IONP will be considered: drug delivery, nanosensors, magnetic resonance imaging (MRI) contrast enhancement and hyperthermia treatments.
220.127.116.11- Drug delivery
Magnetic iron oxide nanoparticle-based nanovectors have been intensively studied also as drug delivery vehicles; this immediately upgrades the MRI imaging probes to theranostic agents that combine both diagnostic and therapeutic elements.[10, 39, 40] One trick is to load IONPs, along with therapeutic agent, into polymer-based matrices. Recently, Nasongkla et al. developed iron oxide nanoparticle-based theranostics, named SPIO-doxorubicin (Dox)-cRGD micelles for synchronous cancer imaging and traceable drug delivery. This approach showed the
therapeutic modality of Doxorubicin and the diagnostic features of the cluster of IONPs which has been co loaded into the cores of PEG-PLA micelles, while the targeting ligand, a cRGD peptide, has been attached onto the micelle surface for targeting the integrin αvβ3 overexpressed on tumor endothelial cells.
The magnetic properties and significant surface area to volume ratio of iron oxide nanoparticles offer desirable characteristics for biomarker detection. Generally, the controlled clustering or aggregation of a few superparamagnetic iron oxide nanoparticles can greatly shorten T2
relaxation time compared to single nanoparticles at the same iron concentration; thus, when magnetic nanosensors aggregate through affinity ligands to the biomarkers, a decrease in the T2
relaxation time is observed, allowing the sensitive and accurate detection of biomarkers with excellent temporal and spatial resolution.[45, 46]
El-Boubbou et al. developed a magnetic nanosensor bearing carbohydrates to screen the carbohydrate-binding characteristics of cancer cells by MRI. The system consists of micro coils for radio-frequency excitation and signal detection, an on-board NMR spectrometer, a portable magnet, and micro-fluidic networks. Magnetic iron oxide nanoparticles were conjugated with antibodies to each biomarker, followed by incubation with samples of cancer cells. Significant differences in T2 relaxation time were observed for a variety of cancer cells using this
system; in this way, this strategy with high sensitivity, specificity and high-throughput shows great potential for early cancer diagnosis in the clinic. 
At the same time, Colombo et al. reported the accurate and reliable detection of anti-HSA (human serum albumin) antibodies by protein-functionalized magnetic nano-spherical probes due to the reversible alteration of their micro aggregation state induced by protein antibody specific interaction, sensed as changes in the T2 relaxation time of surrounding water
18.104.22.168- Magnetic Resonance Imaging (MRI): T2 and T1 contrast agent
The contrast enhancement in MRI occurs as a result of the interaction between the contrast agents and neighboring water protons, which can be affected by many intrinsic and extrinsic factors such as proton density and MRI pulse sequences. The basic principle of MRI is based on nuclear magnetic resonance (NMR) together with the relaxation of proton spins in a magnetic field. When the nuclei of protons are exposed to a strong magnetic field, their spins align
There are two different relaxation pathways: the first, called longitudinal or T1 relaxation, and the
second, called transverse or T2 relaxation.Based on their relaxation processes, the contrast agents
are classified as T1 and T2 contrast agents. Commercially available T1 contrast agents are usually
paramagnetic complexes, while T2 contrast agents are based on IONPs, which are the most
representative nanoparticulate. It is reported in Table.1.1 some examples of T
2 contrast agents
based on IONPs, commonly exploited in biomedical MRI. More detailed information regarding the use of nanoparticles as contrast agents for MRI can be found in chapter II.
Table. 1.1: Commercially available T2 contrast agent based on iron oxide nanoparticles.
Using magnetic nanoparticles, particularly those capable of being delivered selectively to a tumor, offer the potential to deliver site-selective, and even cell-specific, heat to the local or microscopic environment of a tumor. The underlying mechanism is that magnetic nanoparticles can act as antennae in an external alternating magnetic field to convert electromagnetic energy into heat. This feature holds promise in cancer therapy for cancer cells that are more susceptible to elevated temperature than normal cells. In the thermo-therapy, magnetic fluids containing IONPs are delivered to the tumor and then heated by external alternating magnetic field, resulting in an increase of the local temperature of cancer tissue. In this sense, Zhao and co-workers have found that head and neck tumor cells in mice can be killed in half an hour without harming normal cells by injecting a IONPs solution directly into the tumor site under the presence of an alternating magnetic field. In an analogue study aminosilane coated IONPs
15 1.4. Manganese oxide nanoparticles
Manganese (Mn) is one of the most abundant elements in the biosphere. Manganese oxide nanoparticle systems are of interest for a variety of applications including catalysts and electronics. Their magnetic characteristics, like the observation of ferromagnetism in nanoparticulate MnO (which is otherwise a bulk antiferromagnet), have attracted substantial interest in the recent years. The unique electronic configuration of the 3d5 shell of Mn2+ makes
it an excellent magnetic probe for applications in the biomedical field such as drug delivery and biomedical imaging as an MRI contrast agent. Indeed, some colloidal nanoparticles containing
manganese (II) have recently been reported as contrast agents for MRI.
Manganese possesses five unpaired electrons, and the spin of them in manganese perturbs the relaxation of proton in water molecules, which results in an efficient shortening of longitudinal relaxation time, and hence increases the intensity of magnetic resonance signal.
The recent development of molecular and cellular imaging to help visualize disease-specific biomarkers at the molecular and cellular levels has led to an increased interest in magnetic nanoparticles as MRI contrast agents. In particular, superparamagnetic iron oxide (SPIO) has emerged as the prevailing agent so far. However, their negative contrast effect and magnetic susceptibility artifacts are significant drawbacks of using SPIO in MRI. The resulting dark signal can mislead the clinical diagnosis in T2-weighted MRI because the signal is often confused with
the signals from bleeding, calcification, or metal deposits and the susceptibility artifacts distort the background image. In comparison with SPIO, the MnO nanoparticles contribute bright field of T1-weighted MRI, which can be more easily distinguished as they enhance signal instead
of reducing it. As a result, the application of the MnO nanoparticles as contrast agent of MRI has gained considerable attention.
1.4.1. Synthesis of manganese oxide nanoparticles
For this, both the transverse and longitudinal relaxation rates (1/T2 and 1/T1) are measured, and
plotted as a function of the Mn concentration values to calculate their relaxivities (r2 and r1). The
potential of a positive (T1) contrast agent for MRI can be established by high r1 values and r2/r1
values as close as possible to 1.
One of the first studies regarding MnO nanoparticles, performed by Na et al, revealed the strong dependence of the nanoparticle core surface on the longitudinal relaxivity. They developed PEG–lipid-coated MnO nanoparticles with core diameters ranging from 7–25 nm. Unfortunately, very low longitudinal relaxivities were found (r1 = 0.37 mM-1 s-1 and r2/r1 = 4.7 for 7 nm
diameter MnO nanocrystals at 3 T). The rather low relaxivities nonetheless were used to label and to track rat glioma cells in vivo, using T1-weighted imaging sequences. Then, hollow MnO
particles with a ~25 nm thick porous silica shell were designed as high stability cell tracking imaging probes. Compared with the latter, the longitudinal relaxivity of these particles appeared slightly increased (r1 = 0.99 mM-1 s-1 at 11.7 T), allowing the tracking of mesenchymal
stem cells over a period of at least 14 days. However, the longitudinal relaxivity of these suspensions was still four (4) to ten (10) times lower than that observed for common clinical contrast agents such as Gd-DTPA and Gd-DOTA. In fact, coating MnO particles with a layer of silica considerably affects optimal water exchange between the matrix and the surface paramagnetic ions, which is a key mechanism guaranteeing the performance of this kind of MRI contrast agents. Although Mn2+ ions are paramagnetic, MnO nanoparticles in the range 5–10 nm express an antiferromagnetic behaviour. The most significant increase in relaxivity was reported for MnO particles synthesized using polyol techniques (r1 = 7.75 at 1.5 T, for
PEG-coated MnO particles). However, the relaxometric ratio of these particles was close to that of Mn ions (r2/r1 = 10), revealing the possible degradation of MnO cores upon complexation with
carboxylic ligands. Indeed, aqueous Mn2+ solutions show relaxivities in the order of r1 = 5.2 mM -1 s-1 and r
2 = 61 mM-1 s-1 at 1.41 Tesla and 25 ˚C. Hence, the coating strategies are important to
provide enhanced colloidal stability, with possible improvement on the chemical stability of MnO nanoparticles.
1.4.2. Applications of Manganese oxide Nanoparticles in Biomedical Research
Current MRI contrast agents are in the form of either paramagnetic complexes or magnetic nanoparticles. Paramagnetic complexes, which are usually gadolinium (Gd3+) or manganese (Mn2+) chelates, accelerate longitudinal (T1) relaxation of water protons and exert bright contrast
in regions where the complexes localize. For instance, gadolinium diethylenetriamine pentaacetate (Gd-DTPA) has been the most widely used of such complexes and its main clinical applications are focused on detecting the breakage of the blood-brain barrier (BBB) and changes in vascularity, flow dynamics, and perfusion. Manganese-enhanced MRI (MEMRI), which uses manganese ion (Mn2+) as a T
1 contrast agent, is applicable to animals only owing to the toxicity
of Mn2+ when it accumulates excessively in tissues and despite the increasing appreciation of this technique in neuroscience research.
The most commonly used positive (T1-weighted) contrast agent in clinic is gadolinium chelates,
such as the popular Gd-diethylenetriamine pentaacetate (Gd-DTPA) and Gd-tetraazacyclododecanetetraacetic acid (Gd-DOTA). However, the dissociated gadolinium ions from gadolinium chelates could induce the risk of nephrogenic systemic fibrosis (NSF). Thus, many strategies, such as the loading of macromolecules and micelles, the fabrication of nanoscale objects, and so on, have been attempted to inhibit the toxicity and side-effect of released gadolinium ions together with retaining good contrast effect. Especially, the application of inorganic nanoparticles as contrast agent of MRI has gained considerable attention due to relatively high stability and good MRI function. For example, gadolinium compound-based crystalline nanoparticles, such as the Gd-containing nanoparticles of Gd2O3, GdF3 and NaGdF4,
provide a rigid crystal environment that is effectively prevent nanoparticles from releasing free gadolinium ions, and so that they have been mostly investigated as a new generation of positive contrast agents. As mentioned before, the electronic configuration of manganese ions, which has five unpaired electron, results in an efficient shortening of longitudinal relaxation time of proton in water together with the enhancement of magnetic resonance signal intensity. Furthermore, the toxicity of manganese ions is much lower than that of gadolinium ions. As a result, the manganese compound-based crystalline nanoparticles, such as MnO nanoparticles, are expected to become potential positive contrast agents for T1-weighted MRI. It is generally
Therefore, it is essential to synthesize monodisperse ultrasmall MnO nanoparticles to provide large specific surface area for touching water molecules intimately. Since the as-synthesized MnO nanoparticles are generally hydrophobic, surface modification is attempted to render these MnO nanoparticles hydrophilic and more biocompatible.
At present, there is one commercial Mn-based MRI contrast agent, mangafodipirtrisodium (Mn-DPDP), in clinical use. However, Mn-based complexes are easy to dissociate after administration to yield free Mn2+ because of the conversion between the six- and seven-coordinated states,
1. Sperling, R.A., et al., Biological applications of gold nanoparticles. Chemical Society Reviews, 2008. 37(9): p. 1896-1908.
2. Verderio, P., Synthesis and Biofunctionalization of Novel Composite Nanocarriers for
Targeted Detection and Treatment of Malignant Cells, in Chemical Sciences2014,
University of Milan Bicocca: Milan.
3. Ladj, R., et al., Individual inorganic nanoparticles: preparation, functionalization and in
vitro biomedical diagnostic applications. Journal of Materials Chemistry B, 2013. 1(10):
4. Swierczewska, M., S. Lee, and X. Chen, Inorganic nanoparticles for multimodal
molecular imaging. Molecular imaging, 2011. 10(1): p. 3.
5. Peng, G., et al., Diagnosing lung cancer in exhaled breath using gold nanoparticles. Nature nanotechnology, 2009. 4(10): p. 669-673.
6. Yeom, S.-H., et al., Nanostructures in biosensor--a review. Frontiers in bioscience (Landmark edition), 2010. 16: p. 997-1023.
7. Na, H.B., I.C. Song, and T. Hyeon, Inorganic nanoparticles for MRI contrast agents. Advanced Materials, 2009. 21(21): p. 2133-2148.
8. Tan, S., et al., Lipid-enveloped hybrid nanoparticles for drug delivery. Nanoscale, 2013. 5(3): p. 860-872.
9. Kim, C.S., et al., Inorganic nanosystems for therapeutic delivery: status and prospects. Advanced drug delivery reviews, 2013. 65(1): p. 93-99.
10. Huang, H.-C., et al., Inorganic nanoparticles for cancer imaging and therapy. Journal of controlled Release, 2011. 155(3): p. 344-357.
11. Sapsford, K.E., et al., Functionalizing nanoparticles with biological molecules:
developing chemistries that facilitate nanotechnology. Chemical reviews, 2013. 113(3): p.
12. Wilson, D.S., et al., Orally delivered thioketal nanoparticles loaded with TNF-α–siRNA
target inflammation and inhibit gene expression in the intestines. Nature materials, 2010.
9(11): p. 923-928.
13. Pankhurst, Q.A., et al., Applications of magnetic nanoparticles in biomedicine. Journal of Physics D: Applied Physics, 2003. 36(13): p. R167.
14. Xu, C. and S. Sun, Monodisperse magnetic nanoparticles for biomedical applications. Polymer International, 2007. 56(7): p. 821-826.
15. O'Handley, R.C., Modern Magnetic Materials: Principles and Applications. 2000: Wiley & Co. ©, New York (USA).
16. Gupta, A.K. and M. Gupta, Synthesis and surface engineering of iron oxide nanoparticles
for biomedical applications. Biomaterials, 2005. 26(18): p. 3995-4021.
18. Laurent, S., et al., Magnetic iron oxide nanoparticles: synthesis, stabilization,
vectorization, physicochemical characterizations, and biological applications. Chemical
reviews, 2008. 108(6): p. 2064-2110.
19. Jang, J.t., et al., Critical Enhancements of MRI Contrast and Hyperthermic Effects by
Dopant‐Controlled Magnetic Nanoparticles. Angewandte Chemie, 2009. 121(7): p.
20. Figuerola, A., et al., From iron oxide nanoparticles towards advanced iron-based
inorganic materials designed for biomedical applications. Pharmacological Research,
2010. 62(2): p. 126-143.
21. Huber, D.L., Synthesis, properties, and applications of iron nanoparticles. Small, 2005. 1(5): p. 482-501.
22. Skorvanek, I. and R.C. O’Handley, J. Magn. Magn. Mater., 1995. 140: p. 467-469.
23. Ling, D. and T. Hyeon, Chemical design of biocompatible iron oxide nanoparticles for
medical applications. Small, 2013. 9(9‐10): p. 1450-1466.
24. Massart, R., Preparation of aqueous magnetic liquids in alkaline and acidic media. IEEE transactions on magnetics, 1981: p. 1247-1248.
25. Jolivet, J.-P., É. Tronc, and C. Chanéac, Synthesis of iron oxide-based magnetic
nanomaterials and composites. Comptes Rendus Chimie, 2002. 5(10): p. 659-664.
26. Smolensky, E.D., et al., Surface functionalization of magnetic iron oxide nanoparticles
for MRI applications–effect of anchoring group and ligand exchange protocol. Contrast
media & molecular imaging, 2011. 6(4): p. 189-199.
27. Kumfer, B.M., et al., Gas-phase flame synthesis and properties of magnetic iron oxide
nanoparticles with reduced oxidation state. Journal of aerosol science, 2010. 41(3): p.
28. de Castro, V., et al., Functionalisation of Glass with Iron Oxide Nanoparticles Produced
by Laser Pyrolysis. Journal of nanoscience and nanotechnology, 2008. 8(5): p. 2458-2462.
29. Hyeon, T., et al., Synthesis of highly crystalline and monodisperse maghemite
nanocrystallites without a size-selection process. Journal of the American Chemical
Society, 2001. 123(51): p. 12798-12801.
30. Thimmaiah, S., et al., A solvothermal route to capped nanoparticles of γ-Fe2O3 and
CoFe2O4. Journal of Materials Chemistry, 2001. 11(12): p. 3215-3221.
31. Bronstein, L.M., et al., Influence of iron oleate complex structure on iron oxide
nanoparticle formation. Chemistry of Materials, 2007. 19(15): p. 3624-3632.
32. Gage, S.H., et al., Functionalization of monodisperse iron oxide nps and their properties
as magnetically recoverable catalysts. Langmuir, 2012. 29(1): p. 466-473.
33. Luigjes, B., et al., Diverging geometric and magnetic size distributions of iron oxide
nanocrystals. The Journal of Physical Chemistry C, 2011. 115(30): p. 14598-14605.
35. Teng, X. and H. Yang, Effects of surfactants and synthetic conditions on the sizes and
self-assembly of monodisperse iron oxide nanoparticles. Journal of Materials Chemistry,
2004. 14(4): p. 774-779.
36. Jana, N.R., Y. Chen, and X. Peng, Size-and shape-controlled magnetic (Cr, Mn, Fe, Co,
Ni) oxide nanocrystals via a simple and general approach. Chemistry of materials, 2004.
16(20): p. 3931-3935.
37. Huang, J.-H., et al., Investigation of the growth mechanism of iron oxide nanoparticles
via a seed-mediated method and its cytotoxicity studies. The Journal of Physical
Chemistry C, 2008. 112(40): p. 15684-15690.
38. Kim, B.H., et al., Large-scale synthesis of uniform and extremely small-sized iron oxide
nanoparticles for high-resolution T 1 magnetic resonance imaging contrast agents.
Journal of the American Chemical Society, 2011. 133(32): p. 12624-12631.
39. Ho, D., X. Sun, and S. Sun, Monodisperse magnetic nanoparticles for theranostic
applications. Accounts of chemical research, 2011. 44(10): p. 875-882.
40. Yoo, D., et al., Theranostic magnetic nanoparticles. Accounts of chemical research, 2011. 44(10): p. 863-874.
41. Dilnawaz, F., et al., Dual drug loaded superparamagnetic iron oxide nanoparticles for
targeted cancer therapy. Biomaterials, 2010. 31(13): p. 3694-3706.
42. Nasongkla, N., et al., Multifunctional polymeric micelles as cancer-targeted,
MRI-ultrasensitive drug delivery systems. Nano letters, 2006. 6(11): p. 2427-2430.
43. Hwu, J.R., et al., Targeted paclitaxel by conjugation to iron oxide and gold nanoparticles. Journal of the American Chemical Society, 2008. 131(1): p. 66-68.
44. Cheng, K., et al., Porous hollow Fe3O4 nanoparticles for targeted delivery and
controlled release of cisplatin. Journal of the American Chemical Society, 2009. 131(30):
45. Perez, J.M., et al., Integrated nanosensors to determine levels and functional activity of
human telomerase. Neoplasia, 2008. 10(10): p. 1066-1072.
46. Grimm, J., et al., Novel nanosensors for rapid analysis of telomerase activity. Cancer Research, 2004. 64(2): p. 639-643.
47. El-Boubbou, K., et al., Magnetic glyco-nanoparticles: a tool to detect, differentiate, and
unlock the glyco-codes of cancer via magnetic resonance imaging. Journal of the
American Chemical Society, 2010. 132(12): p. 4490-4499.
48. Colombo, M., et al., Femtomolar detection of autoantibodies by magnetic relaxation
nanosensors. Analytical biochemistry, 2009. 392(1): p. 96-102.
49. Brown, M.A. and R.C. Senelka, MRI: Basico Principles and Applications. Magnetic resonance imaging. 2010: Wiley-Blackwell & Co, New York. 661-674.
50. Lee, J.-H., et al., Exchange-coupled magnetic nanoparticles for efficient heat induction. Nature nanotechnology, 2011. 6(7): p. 418-422.
51. Zhao, Q., et al., Magnetic nanoparticle-based hyperthermia for head & neck cancer in
52. Jordan, A., et al., The effect of thermotherapy using magnetic nanoparticles on rat
malignant glioma. Journal of neuro-oncology, 2006. 78(1): p. 7-14.
53. Douglas, F.J., et al., Formation of octapod MnO nanoparticles with enhanced magnetic
properties through kinetically-controlled thermal decomposition of polynuclear manganese complexes. Nanoscale, 2014. 6(1): p. 172-176.
54. Li, J., et al., Understanding the metabolic fate and assessing the biosafety of MnO
nanoparticles by metabonomic analysis. Nanotechnology, 2013. 24(45): p. 455102.
55. Na, H.B., et al., Development of a T1 contrast agent for magnetic resonance imaging
using MnO nanoparticles. Angewandte Chemie, 2007. 119(28): p. 5493-5497.
56. Huang, H., et al., PEGylation of MnO nanoparticles via catechol–Mn chelation to
improving T1‐weighted magnetic resonance imaging application. Journal of Applied
Polymer Science, 2015. 132(31).
57. Chevallier, P., et al., Tailored biological retention and efficient clearance of pegylated
ultra-small MnO nanoparticles as positive MRI contrast agents for molecular imaging.
Journal of Materials Chemistry B, 2014. 2(13): p. 1779-1790.
58. Shin, J., et al., Hollow manganese oxide nanoparticles as multifunctional agents for
magnetic resonance imaging and drug delivery. Angewandte Chemie International
Edition, 2009. 48(2): p. 321-324.
59. Huang, H., et al., Fabrication and evaluation of tumor-targeted positive MRI contrast
agent based on ultrasmall MnO nanoparticles. Colloids and Surfaces B: Biointerfaces,
24 CHAPTER II
MAGNETIC RESONANCE IMAGING
Magnetic Resonance Imaging (MRI) is a technique of generating images used in medical field for diagnostic purposes, based on the physical principle of nuclear magnetic resonance. This technique exploits the magnetic properties of the nuclei with an odd mass number, such as protons, which have an unpaired spin. The spin is a fundamental property in nature (as charge and mass) and it is present in each elementary particle. It is identified by a multiple of ½ and can be positive (+) or negative (-). The spins tend to pair and in an atom with a pair number of elementary particles; they cancel each other. Some substances have different orbital at the same energy level, which are filled with an electron at a time, all with parallel spin, creating paramagnetic materials (substances with unpaired electronic spins which possess magnetic properties). Each spin has an intrinsic angular momentum (vector often indicated by I) which provides a magnetic moment (µ) generated by the rotation of the atomic nuclei on themselves. The magnetic moment is given by the equation:
𝜇 = 𝛾𝑰, eq. (2.1)
where γ is the gyromagnetic ratio, a constant that for hydrogen it has the value of 46.2 MHz/T. The spin can be seen as the rotation of a particle around its own axis and its precession around the axis of the magnetic field B0 (Fig. 2.1). In MRI the unpaired spin of the hydrogen proton (H)
is used to generate images, mainly because of its abundance in the body, which are found for example in water (H2O) and in the fat (-CH2).
Fig. 2.1.Spins align parallel or antiparallel to the magnetic field and precessing as Larmor frequency (ω0).
When the nuclei of the protons are exposed to a strong magnetic field B0, their spins are oriented
𝜔0 = 𝛾𝑩0, eq. (2.2)
where ω0 (Hz) is the resonance frequency of protons in a specific field and B0 [T] is the external
magnetic field. This phenomenon is called proton precession.
When the nuclei are subjected to a resonance frequency in the range of radio frequency (RF), the protons absorb energy and are excited to the antiparallel state. Eventually a small excess of spin will occupy the orientation along the magnetic field, since that’s the state with lower energy. This will create a net magnetization, M, sum of all spins. This net magnetization accumulates in a few seconds up to reach its maximum value (Fig. 2.2). The time it takes depends on the strength of B0 and the examined tissue type or, more specifically by the mobility of protons
within the tissue. When the RF pulse stops, the excited nuclei relax and return to their equilibrium values.
There are two different relaxation pathways occurring at different speeds. The relaxation occurs along both the z-axis and the xy plane and are respectively called R1 (1/T1) and R2 (1/T2), where
T1 or longitudinal relaxation time regards the increase of the net magnetization (Mz) on the
z-plane, while the T2 or transverse relaxation time, involves the decrease of the magnetization in
the perpendicular plane Mxy.
Fig. 2.2.Magnetization vectors during the RF pulse. α will reach the maximum value while φ different levels in the
When an RF pulse is applied to the spin, it generates a transverse magnetization in the xy plane (Mxy) perpendicular to the direction of the static magnetic field. The net magnetization M, as a
Fig. 2.3.Change of spin after the RF pulse .
The change in Mz is due to energy transfer, while that in Mxy is due to the process of spin
dephasing caused by the randomization of the magnetization of excited spins with the same phase coherence immediately after the application of the RF pulse.
Inhomogeneities of the magnetic field can be present as the magnetic properties of an object can cause phase incoherence. The spin-spin interaction between the nuclei of hydrogen or electrons causes a loss of transverse coherence, which produces the real and characteristic relaxation time T2 of the tissues. Therefore, the transverse relaxation time is influenced by inhomogeneous
magnetic fields produced from tissue-inherent factors or from external sources, and the total relaxation time T2*, is described by equation 2.3:
1 𝑇2 ∗=
𝑇2+ 𝛾𝑩𝑠, eq. (2.3)
where γ Bs represents the relaxation caused by the inhomogeneities of the magnetic field and is
called magnetic susceptibility.
2.1 Relaxation times T1 and T2
The longitudinal relaxation time (T1) is characterized by the time it takes to re-align the spins
along the Z axis (Mz) after the RF pulse ceases and returns to approximately 63% of their
equilibrium value M0 (Fig. 2.4.a) . It is defined by equation 2.4.
Fig. 2.4. a) Increased magnetization along the z axis. b) Decay of the magnetization in the xy plane.
On the other hand, the transverse relaxation time (T2) is the time it takes the component of
magnetization to decay in the plane Mxy (Fig. 2.4.b) and is described by the equation:
𝑀𝑥𝑦(𝑡) = 𝑀𝑥𝑦(0)(𝑒 −𝑡
⁄ ), eq. (2.5)
Assuming that protons are exposed to the external static magnetic field B0, after the RF pulse, the
Mxy component returns to steady state and this depends only on the relaxation process. The
phenomenon measured by a coil in the xy plane will cause the decay of the curve and can be compared to a sinusoidal curve (Fig. 2.5)
Fig. 2.5.Signal decay over time. 
Usually the relaxation time T2 is 5-10 times faster than the T1 due to the phase shift. The phase
shift is the randomization of the magnetization vectors and the spins excited with the same phase coherence after the RF pulse. The phase shift occurs due to the inhomogeneity of the magnetic field ΔBz which are created by the magnet in the MR instrument or by internal inhomogeneities caused by the same spin. Since the spins can orient themselves with B0 or away from this, every
spin influence its neighbor. Also the proton interactions with macromolecules, such as proteins or contrast agents in the tissue, can induce local changes of the magnetic field. Perturbations in the magnetic field will cause differences in the precession frequency of spin where B0 will be
instead B0 + ΔB. The difference in frequency will cause an initial phase shift of the spins after
the RF pulse. Since the net magnetization Mxy is the sum of all the vectors for all spins, when
T2 depends on how fast protons in tissue lose their phase coherence and it is associated with their
density. High density means more spin-spin interactions and faster phase shift (Table 2.1). Fluids for example have relatively long distances between molecules and therefore long T2.
Table.2.1: T1 and T2 properties for three different types of tissues.
The characteristics T1 in a tissue have to do with the efficiency of proton transfer. Experimental
data have shown that the transfer of the proton energy will be more efficient when the vibration/rotation frequencies of the molecules are similar to those of Larmor.
As shown before, the Larmor frequency depends on the magnetic field (eq. 2.2), while the vibrational frequencies depend on the physical state of the tissue. Water vibrations cause fluctuations of the protons at the same frequency of the magnetic field and this disturbance in the magnetic field stimulates the relaxation. The natural rotational frequency for fat between the natural C-C bonds is close to the Larmor frequency and therefore has efficient transfer of energy. The opposite occurs for small water molecules that vibrate at much higher frequency leading to a lower energy transfer (Tab. 2.2)
29 2.1.1. T1-weighted images and Repetition Time (TR)
To be able to create a T1-weighted image, the site of interest must be excited several times. The
time between two consecutive RF pulses is defined as Repetition Time (TR) and it directly affects the T1 contrast due to it regulates the amount of time available for relaxation after the
pulse. A long TR allows a better realignment along the z axis and a bigger angle to overturn a radio frequency. Choosing a short TR will highlight tissues with short T1, which will be able to
recover at a higher level. This will give a bigger net magnetization which gives a brighter spot to the image. On the other side, tissues with longer T1 will not have much time to relax and
consequently they will have a smaller net magnetization. This type of image with short TR contains more information about T1 and is therefore called T1-weighted. 
2.1.2. T2-weighted images and echo time (TE)
The echo time (TE) is the time between the RF pulse and the measurement and it has a direct influence on the T2 contrast. By choosing a TE of the same order of magnitude of the T2 of the
tissue, it will underline differences in the relaxivity. Tissues with short T2 will be more phase
shifted and they will lose much of their net magnetization Mxy, while tissues with long T2 will
still have a strong signal. Since a short T2 will give a faster phase shift and a faster signal loss,
tissues with short T2 will appear darker. The greater the difference between the decay curves, the
result will be a sharp and clear contrast (Fig. 2.6). For this reason, T2 contrast agents are
designed in order to increase these differences. Images acquired with a long TR and a long TE will give a dark spot for tissues with short T2 (Tab. 2.2) and are called T2-weighted images.
30 2.1.3 Magnetic Susceptibility
All materials acquire a certain degree of magnetization when subjected to a magnetic field. The magnetic susceptibility is a measure of how much a material can be magnetized and is defined by M = χH where M is the magnetization and H [A/m] the field.
Ferromagnetic materials, normally magnets, are permanently magnetized because of their small magnetic domain where all the magnetic moments are aligned. The domains themselves are randomly oriented one to another causing a cancellation of the magnetization of the entire material. When the latter is subjected to an external magnetic field, the domains align with this and the material becomes permanently magnetized.
Paramagnetic substances instead become magnetized when an external magnetic field is applied but they lose their magnetization when the magnetic field is interrupted. Materials with a large number of unpaired spin, for example gadolinium with seven unpaired electrons, are highly paramagnetic. Following the external magnetic field, the magnetic moments of these unpaired spin create a net magnetization when oriented (Fig 2.7).
Fig. 2.7: Magnetic Behaviors (Magnet Energy Corporation ®)
The resulting rapid fluctuations in the direction of the magnetization lead to a zero mean, therefore, the material behaves similar to a paramagnetic, with the exception that there are no changes at the level of each individual atom but the direction around the crystal changes. Under the influence of an external magnetic field, the magnetic moment of the entire crystal will align with this by giving the material a susceptibility from 100 to 1000 times stronger.
2.2. MRI contrast agents based on magnetic nanoparticles
Among the currently existing imaging techniques such as x-ray, ultrasound, radioactive markers; MRI is the most used diagnostic tool since compared to the other it has the following advantages:
- Production of images with high spatial resolution that allow discriminating tissues according to their biochemical composition.
- Safety for the patient since it is not subjected to ionizing radiation or radioactive isotopes
However, the main limitations are:
- Costs and time required for image acquisition
- Difficulties in the differentiation of tissues magnetically similar but histologically different (healthy tissue from diseased tissue).
These limitations can be overcome by the use of contrast agents which shorten the relaxation times of the spins of the water molecules of the desired tissue and increase the contrast with the surrounding tissues, thus obtaining high-quality images.
Most of the contrast agents commercially available are constituted by paramagnetic complexes. Their first clinical applications were directed to identify the breakage of the blood brain barrier (BBB), changes in the vasculature, flow changes and perfusion. Recently, several studies have been carried out in order to develop new contrast agents for MRI based on magnetic nanoparticles, which are composed by a magnetic and its appropriate surface coating.
Nanostructured contrast agents for MRI are formed from three parts (Fig 2.8):
1) The nanoparticle core which generates the signal increase.
2) The shell, which makes the nanoparticle dispersible in water and thus stable in a biological environment.
3) The bioactive material required for a specific targeting.
Fig. 2.8: Structure of a nanostructured contrast agent.
2.2.1 Surface biocompatibility
For many biomedical applications, in particular for in vivo imaging, nanoparticles should have good colloidal stability and low toxicity in a biological environment. Although there have been synthesized magnetic nanoparticles of high quality with uniform size and high crystallinity by thermal decomposition of metal precursors in organic media, these are hydrophobic, and consequently are not stable in an aqueous environment for biomedical applications. Surface
modification of these nanoparticles is essential to give them hydrophilic properties so that they can be widely used for various biomedical applications. In addition, surface modification is required to increase the functions of the nanoparticle since it is possible to conjugate bioactive material through reactive groups exposed on the surface.
Between the different methods of surface modification currently existing, the more representative strategies are:
Nanoparticles in organic solvents are stabilized by surfactants that have their hydrophilic groups bound to the surface of the nanoparticles and the hydrophobic hydrocarbon tails toward the solvent. Since the atoms on the nanoparticles surface have affinity towards the functional groups, surface functionalization with suitable hydrophilic binders allows the phase transfer of the nanoparticles from organic solvent to aqueous media.
This ligand-exchange method has several advantages such as the simple procedure, passivating thin layer and overall small size. Metal oxide nanoparticles have little reactive surfaces when compared to other types of nanoparticles as there are a limited number of functional groups available. This has prompted research towards strong ligand systems in particular for iron oxide nanoparticles. For example, dopamine has been used as a binder to immobilize functional molecules in iron oxide nanoparticles, while Peng and co-workers have taken advantage of the interactions between hydroxamic acid and iron oxide. Cheon and co-workers have been able to synthesize water-dispersible iron oxide nanoparticles using 2,3-dimercaptosuccinic acid (DMSA), which has a bidentate carboxyl group. The resulting iron oxide nanoparticles are water dispersible and have been successfully used for MRI. To improve nanoparticles biocompatibility, the ligands skeleton is designed to contain biocompatible polymers, such as poly (ethylene glycol) (PEG). Ligands of derivatized phosphine oxide with PEG (PEG-PO) consist of a biocompatible tail of PEG, and a phosphine oxide head coordinated on the nanoparticles surface allowing stabilizing different types of nanoparticles in aqueous media. Polymeric ligands or dendrimers have also been used for the stabilization of iron oxide nanoparticles in aqueous media resulting from their multiple functional groups and bulky structures.